Crumb Rubber Modified Asphalt Concrete for Low Noise ?· Crumb Rubber Modified Asphalt Concrete for…
Post on 05-Jun-2018
Information about research of the paper
Information about research of the paper
Crumb Rubber Modified Asphalt Concretefor Low Noise Surfaces
Massimo Losa, Pietro Leandri, Patrizia Rocchio
University of Pisa, Department of Civil Engineering (DIC)Largo Lucio Lazzarino, 1 56122 Pisa (Italy)
email@example.com, firstname.lastname@example.org, email@example.com
ABSTRACT. The principal advantage of introducing some percentages of crumb rubber inproduction of asphalt mixtures is related to pavement environmental sustainability, since thisprocess allows to recycle a significant amount of an industrial waste and, in some specificcases, to reduce tire/road noise emissions; there are some other not unanimously recognizedadvantages related to this process that are the improvement of asphalt mixture mechanicalproperties and durability as well as friction on pavement surface. This paper reports on aresearch project carried out to evaluate the advantages of using crumb rubber inconstruction of low noise gap graded asphalt concrete surfaces, specifically designed toreduce rolling noise by optimizing surface texture. The study also aimed to define themechanical and functional performances of the mix obtained by using the wet process inorder to assess its potential for use as viable alternative to other low noise asphalt surfacesaimed to improve pavement sustainability by reducing environmental, social and economicimpacts. Results of laboratory and on site tests, carried out on one specifically built fieldtrial, clearly show this mix can have optimal mechanical and functional performance as wellas it can reduce tire/road noise and warrant greater durability of wearing layers; thisconsidering, crumb rubber modified asphalt concrete can be classified as a constructionmaterial that can enhance the three dimensions of sustainability.
KEYWORDS: environmental sustainability, low noise asphalt surface, wet process, crumbrubber, pavement sustainability
2 Crumb Rubber Modified Asphalt Concrete for Low Noise Surfaces
Scrap tires form a major part of the worlds solid waste management problem;in addition, market groups forecast that in the next years post consumer tires willincrease. At the same time, the increasing demand for road transportation hascaused serious problems of noise pollution due to vehicular traffic.
These are only two of the problems resulting from the continuous increase intransportation demand, which has prompted the international scientific communityto search for innovative solutions that allow to use crumb rubber tire in asphaltpavements.
The advantage of using crumb rubber in the production of asphalt mixtures isnot limited to the improvement of road sustainability, but it can be related to animprovement of mechanical properties or a reduction of noise emissions, inaddition an increase of friction (,  and ). At the present time, theinternational scientific community is not unanimous in judging the positive effectsof crumb rubber in terms of reduction of noise emission. According to Sandbergand Ejsmont  there is no evidence that the insertion of small quantities of crumbrubber within asphalt mixtures can allow to significantly reduce tire/road noise.
The use of crumb rubber in asphalt pavements dates back to many years ago (and ). In the Wet process, crumb rubber and bitumen are mixed and left to reactat high temperatures: the final result is known as Asphalt Rubber (AR) (, and ). The AR is used as a modified bitumen in the production of porous asphaltconcretes (open graded) and gap graded asphalt concretes characterized by binderpercentages ranging between 7 and 9%, to which corresponds a crumb rubberpercentage of 1 1.5% on the mixture weight. Moreover, for the need of allowingthe reaction between bitumen and crumb rubber (,  and ), in the Wetprocess it is necessary to use specific mixers for production of the modified asphaltat high temperatures.
This paper reports on research conducted to evaluate the feasibility of using ARin the construction of low noise gap graded asphalt surfaces. The study also aimedto define the mechanical and functional performances of the resulting mix in orderto assess its potential for use as a viable alternative, in terms of environmentalcompatibility and costs, to low noise open-graded asphalt surface. This mix allowsoptimal mechanical and functional performance, it reduces tire road noise andguarantees greater durability of wearing layer performance; in addition, it isenvironmentally friend, by offering a better life-cycle assessment for scrap tire.
Crumb Rubber Modified Asphalt Concrete for Low Noise Surfaces 3
2. Use of crumb rubber modifier in asphalt mixes
The material widely used in vehicle tires is Styrene-Butadiene-Rubber (SBR)that is a synthetic rubber copolymer consisting of styrene and butadiene. It hasgood abrasion resistance and good aging stability when protected by additives;crumb rubber used in this study comes from mechanical grinding of scrap tires atroom temperature; they are represented by 50% by weight of truck tires and 50%by weight of car tires. Figure 1 represents size gradation of crumb rubber used toproduce gap graded mix, according to the wet processes, overlaid to the typicalCRM gradations for production of the Asphalt Rubber. The size gradation of crumbrubber fulfils the requirements of CRM for the production of Asphalt Rubber .
0.01 0.10 1.00 10.00
Sieve size [mm]
Typical Gradation -CRM for AR
Figure 1. The size gradation of crumb rubber
3. Description of experiment
The experiment involved a first step of mix design to define the aggregate grainsize distributions and the optimum asphalt contents to be used in the mix; in thesecond step, laboratory tests were carried out to evaluate mixture performance.
The gap graded asphalt mixture produced by the wet process, was utilized for asurface layer, 3 cm thick, laid on a roughly 150 m long test section within theLeopoldo research project . This project has the specific aim of improvingroad safety and environmental compatibility.
Cores were taken from pavement to check the compliance with the designmixture in terms of aggregate gradation, asphalt content and air void percentage.The in-situ characteristics of the mixture was substantially the same of thelaboratory mixture with regard to the aggregate gradation and the bitumen content;
4 Crumb Rubber Modified Asphalt Concrete for Low Noise Surfaces
as far as the air void contents of in situ mixture, they were approximately 2% morethan the air void contents of the laboratory mixture.
This asphalt wearing course was then evaluated in terms of surfacecharacteristics (friction and texture) and acoustic performance.
4. Mix design
Mix design was carried out by the volumetric method. The optimum asphaltcontent was identified by optimizing the air void contents.
4.1. Aggregate gradation
Physical properties of aggregates, determined according to the UNI-EN 1097-6/7 procedures, are shown in Table 1.
Physical proprieties Basalt 4/6 Sand Mineral Filler
Bulk Specific Gravity
(kg/m3)2753 2629 2650
Apparent Specific Gravity
(kg/m3)2863 2690 2650
(%)1.39 0.86 0.00
Table 1. Asphalt binders characteristics
Sieve size [mm - raised to 0.45 power]
5 2 4
Figure 2. Aggregate size gradation
Crumb Rubber Modified Asphalt Concrete for Low Noise Surfaces 5
The grain size distribution of the studied mixture respects the aggregategradation required by the project specifications for gap graded asphalt mixtureswith the maximum aggregate size equals to 8.0 mm (Figure 2).
The resulting internal structure of the mixture determined by the discontinuousaggregate grading curve can be appreciated in Figure 3.
Figure 3. Internal structure of the mixes
4.2. Optimum asphalt content and volumetric properties of the mixture
The aggregates were mixed with Asphalt Rubber (AR) (Table 2), consisting of20% CRM by weight of binder and the remaining 80% of 50-70 penetration gradebitumen. The optimum asphalt content of the mix was determined by gyratorycompaction, assessing the volumetric characteristics of four mixtures with asphaltcontents ranging from 7.5% to 9.0% (Table 3).
In determining the volumetric properties of the mixes, the aggregate absorptionpercentage was assumed to be equal to 1/3 of water absorption, as required by UNIEN 12697-5.
From the mix design it is possible to determine the optimum percentage ofbitumen capable of minimizing the void percentage and guaranteeing at thecompaction level Nmax a void volume higher than 2% and at the compaction levelNdesign a void volume ranging between 3 5%. From the results obtained it wasselected the optimum bitumen content equal to 8.5%.
6 Crumb Rubber Modified Asphalt Concrete for Low Noise Surfaces
Unit Value Reference
Penetration at 25 C Dmm 25 55 UNI EN 1426
Softening point, Ring & Ball C 58 UNI EN 1427
Fraass breaking point C -7 UNI EN 12593
Flash Point C 250 EN ISO 2592
Elastic recovery at 25 C % 70 UNI EN 13398
Resistance to hardening RTFOT (163 C UNI EN 12607-1)
Loss in mass % 0.5 UNI EN 12607-1
Retained penetration at 25 C % 45 UNI EN 1426
Increase in softening point C 12 UNI EN 1427
Table 2. Physical properties of aggregates
Ninitial=10 14.00 25.98 46.13 2191 2547 74.02 11.98
Ndesign=50 6.81 19.79 65.60 2374 2547 80.21 12.99
Nmax=130 3.95 17.33 77.21 2446 2547 82.67 13.38
Ninitial=10 13.01 26.30 50.51 2191 2519 73.70 13.28
Ndesign=50 5.85 20.22 71.09 2372 2519 79.78 14.38
Nmax=130 3.02 17.83 83.06 2443 2519 82.17 14.81
Ninitial=10 12.19 26.44 53.90 2197 2502 73.56 14.25
Ndesign=50 5.01 20.43 75.47 2377 2502 79.57 15.42
Nmax=130 2.17 18.05 87.96 2448 2502 81.95 15.88
Ninitial=10 11.70 26.86 56.43 2195 2486 73.14 15.16
Ndesign=50 4.54 20.92 78.31 2373 2486 79.08 16.39
Nmax=130 1.71 18.58 90.80 2443 2486 81.42 16.87
NOTE: AC, asphalt content as percentage of mass of aggregates; VA, air voids; VMA, voids in mineral
aggregate; VFA, voids filled with asphalt; Gmb, bulk density of the compacted mixture; Gmm,
maximum density of the mix; VG, volume of aggregate, the bulk volume including the aggregate
pores; VB, volume of effective asphalt binder.
Table 3. Volumetric properties of the mixes
Crumb Rubber Modified Asphalt Concrete for Low Noise Surfaces 7
In Figure 4 the gyratory densification curve of the studied mixture is comparedto the curves obtained for a dense asphalt concrete 0/8 mm (DAC 0/8) with 5.5%bitumen (50-70 penetration grade pure bitumen) and for a stone mastic asphalt 0/8mm (SMA 0/8) with 7.2% bitumen (50-70 penetration grade polymer modifiedasphalt). The results show that the curve referring to the studied mixture has aslight steeper slope and a higher density than the curves referring to the DAC 0/8and SMA 0/8. This highlights that, at the same compaction temperatures, thestudied mixture shows better compaction properties as compared to DAC 0/8 and toSMA 0/8.
1 10 100 1000
Number of Gyrations
Crumb rubber modifiedasphalt concrete
Figure 4. The gyratory densification curves of the studied mixture
5. Mechanical characteristics of the mixture
In order to characterize the mix from a mechanical point of view, IndirectTensile Strength Tests, Resilient Modulus Tests and Fatigue Resistance Tests werecarried out on specimens compacted by the Gyratory Compactor at Ndesign. Theseparameters allow to check both the compliance of the mixture with nationalspecifications for wearing courses and to compare performance of AR withpolymer modified asphalt. Considering the reduced thickness of the layer (30 mm),the rutting performance was neglected.
8 Crumb Rubber Modified Asphalt Concrete for Low Noise Surfaces
5.1. Indirect tensile strength
Indirect Tensile Strength (ITS) measurements were carried out at thetemperature of 25C, according to UNI EN 12697-23. ITS values (Table 4) arehigher than the minimum values required by the national standards for gap gradedasphalt mixes to be used as wearing courses. To evaluate moisture susceptibility,the Indirect Tensile Strength Ratio (ITSR) according to UNI EN 12697-12 wasdetermined. This is represented by the ratio between ITS of samples afterconditioning in water (ITSw) and ITS of unconditioned samples (ITSd). The resultsobtained (Table 4) clearly show that no problems pertaining to moisturesusceptibility arise for the studied mix.
Mechanical properties Specifications
ITSd at 25C
ITSw at 25C
ITSd at 25C
1 0.70 0.62
2 0.70 0.73
3 0.78 0.69
Mean value 0.73 0.68 93.6 0.60 75
St. Dev. 0.05 0.06
COV (%) 6.4 8.2
Table 4. Indirect tensile strength test results
5.2. Resilient modulus
In order to evaluate mix stiffness, the laboratory resilient modulus (MR) wasdetermined by the indirect tensile test on cylindrical specimens (IT-CY) accordingto UNI EN 12697-26 Annex C procedure. MR values of the studied mix are shownin Table 5 together with values determined on specimens of a stone mastic asphalt0/8 mm (SMA 0/8), containing 7.2% bitumen (50-70 penetration grade polymermodified asphalt) and compacted according to the same procedure at Ndesign.Results obtained by the studied mix showed an increase of 50% in MR mean valuescompared to the SMA 0/8. This increase can be explained by the greater stiffness ofAsphalt Rubber binder as compared to polymer modified asphalt binder.
5.3. Fatigue resistance
The fatigue resistance was determined by the Indirect tensile test on cylindricalspecimens (IT-CY) according to UNI EN 12697-24 Annex E. Tests have beencarried out at the temperature of 20C and at a load repetition time equal to 500 ms.
Crumb Rubber Modified Asphalt Concrete for Low Noise Surfaces 9
Figure 5 shows the plot of fatigue resistance curve for the studied mixturetogether with fatigue resistance curve determined on specimens of a stone masticasphalt 0/8 mm (SMA 0/8), containing 7.2% bitumen (50-70 penetration gradepolymer modified asphalt). The studied mixture shows fatigue resistance curvealmost overlapping with SMA 0/8. This means that Asphalt Rubber binder showsfatigue attitude similar to that of modified asphalt binder. In particular the studiedmixture shows a greater fatigue resistance at high strains and a lower fatigueresistance at low strains compared to the SMA 0/8.
Studied mix SMA 0/8
1 3 0.1 124 4 20 3247 2872
2 3 0.1 124 4 20 3521 2020
3 3 0.1 124 4 20 3515 2851
4 3 0.1 124 4 20 3818 1723
Mean value 3525 2367
St. Dev. 233 585
COV (%) 6,6 24,7
Table 5. Resilient modulus test results
y = 2,444.82x-0.24
R = 0.9...